NIR Photoresponse of Perovskite Solar Cells with Titanyl ... ... The effect of titanyl...
Embed Size (px)
Transcript of NIR Photoresponse of Perovskite Solar Cells with Titanyl ... ... The effect of titanyl...
198 © ISUCT Publishing Макрогетероциклы / Macroheterocycles 2019 12(2) 198-201
NIR Photoresponse of Perovskite Solar Cells with Titanyl Phthalocyanine
Vlad V. Travkin, Anton N. Fedoseev, Yury I. Sachkov, and Georgy L. Pakhomov@
Institute for Physics of Microstructures of the Russian Academy of Sciences (IPM RAS), 603950 Nizhny Novgorod, Russian Federation @Corresponding author E-mail: email@example.com, firstname.lastname@example.org
The effect of titanyl phthalocyanine TiOPc in the methylammonium lead triiodide (MAPbI3) perovskite based solar cells is studied. The photovoltaic output of cells at low intensity illumination with lmax= 840 nm is greatly enhanced when using TiOPc as a NIR-absorbing hole conductor. Compared to the reference cells with a standard cuprous iodide CuI as a hole-transporting layer, the photocurrent increases by a factor of 15, so that the narrow-band power conversion efficiency (PCE) exceeds 2 %. It should be pointed out that the irradiation wavelength lies beyond the intrinsic absorption of MAPbI3 or any other material in the device scheme except TiOPc. The improvement is associated with the photoactivity of TiOPc molecules in the near infrared region due to the largely splitted Q-band, as confirmed by the dependence of parameters on the polymorph transition in the TiOPc films.
Keywords: Titanyl phthalocyanine, polymorph transition, NIR absorption, perovskite solar cells.
Влияние фталоцианинового красителя на фотоотклик перовскитных солнечных ячеек в ближней ИК области
В. В. Травкин, А. Н. Федосеев, Ю. И. Сачков, Г. Л. Пахомов@
Институт физики микроструктур РАН, 603950 Нижний Новгород, Российская Федерация @E-mail: email@example.com, firstname.lastname@example.org
Изучено влияние фталоцианина титанила на фотовольтаичские процессы в солнечных элементах на основе трийодида метиламмония-свинца (перовскит MAPbI3). Эффективность преобразования мощности (PCE) в ячейках при освещении низкой интенсивности с максимумом около 840 нм резко возрастает при использова- нии TiOPc в качестве дырочно-транспортного слоя. В сравнении с эталонной ячейкой, содержащей дырочно- транспортный слой йодида меди CuI, фототок увеличивается в 15 раз, так что PCE солнечной ячейки в узком инфракрасном диапазоне превышает 2 %. Следует подчеркнуть, что максимум источника освещения лежит за пределами собственного поглощения MAPbI3 или любого другого материала в схеме устройства кроме TiOPc. Таким образом, прогресс связан с фотоактивностью молекул TiOPc в ближнем инфракрасном диа- пазоне, возникающей из-за сильного расщепления Q-полосы, что подтверждается и зависимостью выходных параметров от полиморфного состояния пленок TiOPc.
Ключевые слова: Фталоцианин титанила, полиморфный переход, поглощение в ближнем ИК диапазоне, перовскитные солнечные ячейки.
Perovkite solar cells have attracted enormous atten- tion in the last decade due to the easily achieved, but still not stabilized, power conversion efficiencies (PCE)
in order of 15–20 % or higher. Planar heterojunction solar cells employing the perovskite/fullerene bilayer were first reported in ref. and since then have aroused great interest among researchers in the field due to the stablizing effect of C60. In these cells, the methylammonium lead triiodide
199Макрогетероциклы / Macroheterocycles 2019 12(2) 198-201
G. L. Pakhomov et al.
(MAPbI3) perovskite is a single, or dominant, photoabsorber which provides the photoconversion activity in the UV/vis- ible range up to ~750 nm. At longer wavelengths the cells are optically inactive. Several approaches to enhance spectral range of perovskite-based cells are reported. So, the pho- toactivity of the perovskite material itself can be extended to the NIR domain by altering its chemical structure, as shown by the example of various formamidium, mixed-metal or mixed-halide derivatives.[3-5] Alternatively, additives to the perovskite precursor solution, like soluble phthalo- cyanines, enhance the light absorption being incorporated in the resulting active layer and thus improve the efficiency of cells. In ref., tert-butyl substituted copper phthalocya- nine not only helped to absorb the incident photons, but also inhibited the formation of unwanted voids in the perovskite structure during the film growth. Eventually, the photon-to- electron conversion diapason of the whole multilayer device can be widened by embedding functional components that are intrinsically photoactive at the wavelengths where the perovskite materials do not absorb.[7,8]
In this work we report on the photovoltaic effect in the MAPbI3-based cells irradiated with a narrow-band light source in the near infrared (NIR). In the reference cell, cuprous iodide CuI was used as hole transporter in conjunction with MAPbI3. The gain in the photoresponse was achieved through pairing MAPbI3 with the molecular hole-transporting layer composed of the NIR photoabsorb- ing dye molecules, TiOPc (titanyl phthalocyanine).
The preparation of the multilayer cells by the vacuum deposition technique is described previously.[9,10] The schematic of cells is shown in Figure 1. Initially, the cell with cuprous iodide CuI as a hole-transporting layer (HTL) were obtained follow- ing the technological concept arisen in Refs.[1,2,9] They served further as a reference. The composition of the cells (thickness in parentheses) was: glass/ITO/MoO3 (3 nm)/CuI (15 nm)/MAPbI3 (250 nm)/C60 (35 nm)/BCP (6 nm)/Ag (50 nm). Here, ITO is a dou- ble indium-tin oxide, MoO3 is a substoichiometric molybdenum trioxide, and BCP is a bathocuproine (exciton blocking layer). The active area of the cells is determined by the strip-like top elec- trodes and equals to 0.13 cm2.
In the next two series, a 30 nm thick titanyl phthalocyanine TiOPc (Aldrich, dye content 95 %) was deposited as HTL in place of CuI. An MoO3 anodic underlayer in these series was omitted
due to incompatibility with the molecular overlayer (very poor electrical quality of the resulting diodes). Probably, the reason lies in the pronounced disordering of TiOPc molecules in films grown on MoO3 (as described, e.g., in ref.)which makes them discontinu- ous. In the first series, the as-deposited TiOPc layer was used, while in the second series the molecular layer underwent thermal treatment at 150 oC during 10 min in air after deposition. All other experimen- tal conditions and processes were strictly identical to those used for manufacturing and testing of the reference cells with CuI.
Photoelectrical measurements were carried out in a shielded steel chamber filled with the ultrapure argon at room temperature. A NIR LED delivering the incident light power Pin of 2 mW/cm2 was used to irradiate the samples, its emission spectrum is shown in Figure 1. The J-V curves were taken with a Keithley SCS-4200 parameter analyzer. Note, there was no irradiation of samples in the UV and visible range, all measured photovoltaic parameters correspond to the narrow-band irradiation within the emission peak shown in Figure 1. The optical transmission of samples in the range of 360–960 nm was measured using a FireFly4000 spectrometer.
Results and Discussion
Figure 2(a) compares the intrinsic optical absorption of TiOPc layer on glass/ITO before and after annealing. The larger splitting of Q-band in annealed samples indi- cates the stronger aggregation of molecules in solid state. It is well-known that polycrystalline vacuum-deposited TiOPc films exist in, at least, two temperature polymorphs. [11-15] The room-temperature polymorph is ascribed as phase I (or β), the high-temperature one – as phase II (or α). All polymorphic modifications of TiOPc are extensively studied in the literature. The TiOPc molecule has a non-planar, convex shape with axial oxygen atom at the top (Figure S1). Monoclinic β-TiOPc can be viewed as an ensemble of alternating layers of faced Pc-rings and parallel Ti=O bonds (TOC Figure), while in triclinic α-phase the stacks of slipped molecules have the Ti=O bonds oriented in oppo- site directions with alternating downward and upward axial ligands.[11,12,15] The latter arrangement determines much higher photoconductivity in the α-TiOPc crystals and thin films.[14,15] Several groups[11,13] reported on the beneficial effect of β-to-α transition on the photovoltaic parameters of the devices employing the TiOPc-based molecular het- erojunctions.
In our previous work we have studied the wavelength- selecti